- Thermal spraying
Thermal spraying techniques are
coatingprocesses in which melted (or heated) materials are sprayed onto a surface. The "feedstock" (coating precursor) is heated by electrical (plasma or arc) or chemical means (combustion flame).
Thermal spraying can provide thick coatings (approx. thickness range 20 micrometres - several mm, depending on the process and feedstock), over a large area at high deposition rate as compared to other coating processes such as
electroplating, physical and chemical vapor deposition. Coating materials available for thermal spraying include metals, alloys, ceramics, plastics and composites. They are fed in powder or wire form, heated to a molten or semimolten state and accelerated towards substrates in the form of micrometre-size particles. Combustion or electrical arc discharge is usually used as the source of energy for thermal spraying. Resulting coatings are made by the accumulation of numerous sprayed particles. The surface may not heat up significantly, allowing the coating of flammable substances.
Coating quality is usually assessed by measuring its
porosity, oxide content, macro and microhardness, bond strengthand surface roughness. Generally, the coating quality increases with increasing particle velocities.
Several variations of thermal spraying are distinguished:
High-velocity oxygen fuelspraying (HVOF)
*Wire arc spraying
Flame, wire-arc and plasma spraying
In classical (developed between 1910 and 1920) but still widely used processes such as flame spraying and wire arc spraying, the particle velocities are generally low (< 150 m/s), and raw materials must be molten to be deposited. Plasma spraying, developed in the 1970s, usesa high-temperature plasma jet generated by arc dischargewith typical temperatures >15000 K, which makes itpossible to spray refractory materials such as oxides, molybdenum, etc.
High velocity oxygen fuel spraying (HVOF)
During the 1980s, a class of thermal spray processes called
high velocity oxy-fuel sprayingwas developed: A mixture of fuel and oxygen is fed into a combustion chamber, where they are ignited and combustedcontinuously. The resultant hot gas at a pressure close to 1 MPa emanates through a converging–diverging nozzle and travels through a straight section. The fuels can be gases (hydrogen, methane, propane, propylene, acetylene, natural gas, etc.) or liquids (kerosene, etc.). The jet velocity at the exit of the barrel (>1000 m/s) exceeds the speed of sound. The process has been most successful for depositing cermet materials (WC–Co, etc.) and other corrosion-resistant alloys (stainless steels, nickel-based alloys, etc.).
In the 1990s, cold spraying (often called cold gas dynamic spraying) has been introduced. The method was originally developed in Russia with the accidental observation of the rapid formation of coatings, while experimenting with the particle erosion of the target exposed to a high velocity flow loaded with fine powder in a wind tunnel. In cold spraying, particles are accelerated to very high speeds by the carrier gas forced through a converging–diverging de Laval type nozzle. Upon impact, solid particles with sufficient kinetic energy deform plastically and bond mechanically to the substrate to form a coating. The critical velocity needed to form bonding depends on the materials properties, powder size and temperature. Soft metals such as Cu and Al are best suited for cold spraying, but coating of other materials (W, Ta, Ti, MCrAlY, WC–Co, etc.) by cold spraying has been reported.
The deposition efficiency is low, and the window of process parameters and suitable powder sizes is narrow. To accelerate powders to higher velocity, finer powders (<20 micrometre) are used. It is possible to accelerate powder particles to much higher velocity using a processing gas having high
speed of sound(helium instead of nitrogen).However, helium is costly and its flow rate, and thus consumption, is higher. To improve acceleration capability, nitrogen gas is heated up to about 900 C. As a result, deposition efficiency and tensile strength of deposits increase.
Is a novel modification of
high-velocity oxy-fuel spraying, in which the temperature of combustion gas is lowered by mixing nitrogen with the combustion gas, thus bringing the process closer to the cold spraying. The resulting gas contains much water vapor, unreacted hydrocarbons and oxygen, and thus is dirtier than the cold spraying. However, the coating efficiency is higher. On the other hand, lower temperatures of warm spraying reduce melting and chemical reactions of the feed powder, as compared to HVOF. These advantages are especially important for such coating materials as Ti, plastics, and metallic glasses, which rapidly oxidize or deteriorate at high temperatures.
*Wear control (
*Repairing damaged surfaces
*Temperature/oxidation protection (thermal barrier coatings)
High Velocity Oxygen-Fuel(HVOF)
Plasma sprayingwith powders under atmospheric and vacuum or low pressure conditions
Thermal spraying need not be a dangerous process, if the equipment is treated with care, and correct spraying practices are followed. As with any industrial process, there are a number of hazards, of which the operator should be aware, and against which specific precautions should be taken.
Ideally, equipment should be operated automatically, in enclosures specially designed to extract fumes, reduce noise levels, and present direct viewing of the spraying head. Such techniques will also produce coatings that are more consistent. There are occasions when the type of components being treated, or their low production levels, requires manual equipment operation. Under these conditions, a number of hazards, peculiar to thermal spraying, are experienced, in addition to those commonly encountered in production or processing industries.
Metal spraying equipment uses compressed gases, which create noise. Sound levels vary with the type of spraying equipment, the material being sprayed, and the operating parameters. Typical sound pressure levels taken 1 meter behind the arc.
Combustion spraying equipment produces an intense flame, which may have a peak temperature more than 3,100°C, and is very bright. Electric arc spraying produces ultra-violet light, which may damage delicate body tissues. Spray booths, and enclosures, should be fitted with ultra-violet absorbent dark glass. Where this is not possible, operators, and others in the vicinity should wear protective goggles containing BS grade 6 green glass. Opaque screens should be placed around spraying areas. The nozzle of an arc pistol should never be viewed directly, unless it is certain that no power is available to the equipment.
Dust and fumes
The atomization of molten materials produces a certain amount of dust and fumes. Proper extraction facilities are vital, not only for personal safety, but to minimize entrapment of re-frozen particles in the sprayed coatings. The use of breathing masks, fitted with suitable filters, is strongly recommended, where equipment cannot be isolated.Certain materials offer specific known hazards.
#Finely divided metal particles are potentially pyrophoric and none should be allowed to accumulate.
#Certain materials e.g. aluminum, zinc and other base metals may react with water to evolve hydrogen. This is potentially explosive and special precautions are necessary in fume extraction equipment.
#Fumes of certain materials, notably zinc and copper alloys are unpleasant to smell, and, in certain individuals, may cause a fever-type reaction. This may occur some time after spraying and usually subsides rapidly. If it does not, medical advice must be sought.
Combustion spraying guns use oxygen and fuel gases. The fuel gases are potentially explosive. In particular, acetylene may only be used under approved conditions. Oxygen, while not explosive, will sustain combustion, and many materials will spontaneously ignite, if excessive oxygen levels are present. Care must be taken to avoid leakage, and to isolate oxygen and fuel gas supplies, when not in use.
Electric arc guns operate at low voltages (below 45 V dc), but at relatively high currents. They may be safely hand-held. The power supply units are connected to 440 V AC sources, and must be treated with caution.
*Topical review "Warm spraying—a novel coating process based on high-velocity impact of solid particles" [http://dx.doi.org/10.1088/1468-6996/9/3/033002 Sci. Technol. Adv. Mater. 9 (2008) 033002 (17 pages)] ("free download")
*Pawlowski L, "The Science and Technology of Thermal Spray Coatings" (New York: Wiley, 1995)
*Papyrin A, Kosarev V, Klinkov S, Alkhimov A and Fomin V "Cold Spray Technology" (Oxford: Elsevier, 2007)
* [http://www.p2pays.org/ref/03/02454/altmeth.htm Alternative Methods of Metal Deposition]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Thermal spraying — Thermal spraying. См. Тепловое распыление. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) … Словарь металлургических терминов
thermal spraying — karštasis užpurškimas statusas T sritis chemija apibrėžtis Dangos gavimas iš aukštatemperatūre dujų čiurkšle purškiamo išlydyto metalo (ar polimero) dalelių, kurios susidurdamos su dengiamu paviršiumi su juo sukimba. atitikmenys: angl. heat… … Chemijos terminų aiškinamasis žodynas
Thermal barrier coating — Thermal barrier coatings are highly advanced material systems applied to metallic surfaces, such as gas turbine or aero engine parts, operating at elevated temperatures. These coatings serve to insulate metallic components from large and… … Wikipedia
heat spraying — karštasis užpurškimas statusas T sritis chemija apibrėžtis Dangos gavimas iš aukštatemperatūre dujų čiurkšle purškiamo išlydyto metalo (ar polimero) dalelių, kurios susidurdamos su dengiamu paviršiumi su juo sukimba. atitikmenys: angl. heat… … Chemijos terminų aiškinamasis žodynas
hot spraying — karštasis užpurškimas statusas T sritis chemija apibrėžtis Dangos gavimas iš aukštatemperatūre dujų čiurkšle purškiamo išlydyto metalo (ar polimero) dalelių, kurios susidurdamos su dengiamu paviršiumi su juo sukimba. atitikmenys: angl. heat… … Chemijos terminų aiškinamasis žodynas
Тепловое распыление — Thermal spraying Тепловое распыление. Группа методов формирования покрытия, в которых дисперсные металлические или неметаллические материалы наносятся в расплавленном или полурасплавленном состоянии. Материал покрытий может быть в форме порошка,… … Словарь металлургических терминов
Vacuum plasmaspraying — (VPS) is a technology for etching and surface modification to create porous layers with high reproductibility and for cleaning and surface engineering of plastics, rubbers and natural fibres as well as for replacing CFCs for cleaning metal… … Wikipedia
List of coating techniques — This list contains an overview of coating techniques for thin film deposition, found in the field of materials science. The techniques can be classified as follows: Chemical vapor deposition (CVD) * Metalorganic vapour phase epitaxy *… … Wikipedia
Plasma Spray — Plasma spraying, a method of thermal spraying, is a materials processing technique for producing coatings and free standing parts using a plasma jet. Deposits having thickness from micrometers to several millimeters can be produced from a variety … Wikipedia
Metalworking — Machining a bar of metal on a lathe. Metalworking is the process of working with metals to create individual parts, assemblies, or large scale structures. The term covers a wide range of work from large ships and bridges to precise engine parts… … Wikipedia